SOLID STATE SPECTROSCOPY
RARE EARTH  HYDRIDE CENTRES IN THE ALKALINE EARTH FLUORIDES
A thesis presented for the degree of Doctor of Philosophy in Physics in the University of Canterbury,
Christchurch, New Zealand.
by
I.T. JACOBS _{� }
THESIS
The white man drew a small circle in the sand and told the red man, "Tbi s is what the Indian knows", and drawing a big circle around the small one, "This is what the white man knows". The Indian took the stick and swept an
immense ring around both circles: "This is where the white man and the red man know nothing."
i
My thanks are due to Professor McLellan for my acceptance as a research student. In particular I wish to thank Dr G.D. Jones for his enthusiastic supervision as well as Professor Batten and Dr K. Zdansky for their continuing interest and many con tributions. Professor B.G. Wybourne's interest in this work has been appreciated together with many helpful discussions with Mr M. Presland.
Thanks are due also to Mr D. Greig for his
patience in the cryogenics room and to Mr R. Ritchie for technical assistance.
Financial assistance has been received from the New Zealand University Grants Committee, and from the United States Air Force Office of Scientific Research under AFOSR Grant No.
127567.
The Grants Committee also provided a Postgraduate Scholarship. Without this assistance this work would not have beenCHAPTER I
CHAPTER II
CHAPTER III
CHAPTER IV
ll
CONTENTS
Introduction
A Review of the Theory
Lattice and Localised Vibrations The Electronic Levels of Ions in
Crystals
The ElectronPhonon Interaction
Experimental Considerations Hydrogenation
Instrumentation
Experimental Results Infrared Spectra Vibronic Levels
CHAPTER V A Discussion of the Infrared Spectra
Part I Vibronic Splittings CeriumHydride Centres
PraseodymiumHydride Centres Neodymium and the Other Rare
Earths
CHAPTER VI
iii
The U.V. Spectra of Cerium in the Alkaline Earth Fluorides
Part I Experimental Results
Cerium Hydrogenic Centres Other Hydrogenic Centres
Part II Analysis of the Cerium Electronic Spectra
Vibronic Transitions
The Isotope and Vibronic Shifts Lattice Vibrations and the
Fluorine Site Vibronic Progressions
. . .
. .
.
. . .
. . .
CHAPrER VII The Point Charge Model for the IsotopeCH.APTER VIII
CHAPTER IX
APPENDIX (I) REFERENCES APPENDIX (II)
and Vibronic Shifts
Possible Extensions to the Models
Praseodymium Optical Spectra PraseodymimHydride Centres The Ground State Multiplet The Electronic Isotope Shifts
Suggestions for Future Work
A Related Problem
iv
LIST OF FIGURES
Figure Page
1 The Harmonic Oscillator in c4v Symmetry 2.5 2 The Tetragonal Site (Re3+
H) 2.7
3
Infrared Absorption Spectra 4.24 High Resolution Local Mode Spectra (Ce3+_{H) } _{4.5 } 5 High Resolution Local Mode Spectra (Pr3+_{H) } _{4.7 } 6 Lines Fitted to Pr3_{+H Local Mode Spectrum } _{4.12 } 7 Low Lying States for Ce3+_{H Centre } _{5.2 } 8 Low Lying Electronic Pr3+ _{Levels } _{5.9 } 9 Splitting pattern of (Pr3_{+H) (xy) Local Mode } _{5.15 } 10 Cerium (3+) Electronic Energy Scheme 6.2 11 ce3+_{F} _{Tetragonal Site Absorption in CaF2 } _{6.3 }
12 Ce3+_{F} _{Fluorescence in CaF2 } _{6.6 }
13 Ce3+_{F} _{Fluorescence in SrF2 }
14 Low Resolution Ce3+ _{U.V. } _{Absorption Spectra } 15 U.V. ce3+_{H:D Absorption Spectra }
16 U.V. Ce3+_{H:D Fluorescence Spectra }
17(a,b) U.V. Site (Ce+H?) Absorption Spectra
18 Infrared Absorption Spectra Showing U.V. Site Line
19 CeriumHydride Centre Vibronic Progressions
20 Pr3+ _{Energy Levels }
21 Praseodymium Optical Absorption Spectrum
22 Praseodymium Optical Fluorescence Spectrum
6.7 6.11 6.12 6.14
6.19
6.20 6.41 8.2 8.4
V
Figure Page
23 Energy Level Diagram for the Tetragonal Pr3+_H:D
24
25
A1Sites
Cubic Field Splitting of the 3
H4 Multiplet
Splitting of the Pr3+_{}3_{P1 } _{Levels }
Gd3+_{}_{H Absorption Spectra }
vi
LI ST OF TABLES
Table Page
1 Relative Intensities of the Infrared Absorption
2 3 4 5
Lines
Multiplication Table of the
c
_{4v Double Group } Infrared Absorption DataCerium Vibronic Levels
Praseodymium Vibronic Levels
6 Tetragonal Ce3+_{F} _{Centre Vibronic Progression } Intervals
7(a,b) Tetragonal Ce3+
F Centre Data in CaF2, SrF 2 and BaF 2
8(a,b) CeriumHydride Tetragonal Centre Lines (a) Absorption, (b) Fluorescence
9
Cerium_{}Hydride Centre Electronic Lines1 0 Sign and Ratio of Cerium Electronic Isotope Shifts
11(a,b) CeriumHydride Centre Vibrational Intervals in CaF 2 and SrF 2
12 Assignment of the Lattice Vibrational Intervals in Calcium Fluoride
13 14 15
Praseodymium Absorption Data Praseodymium Fluorescence Data
Pr3+_{}_{D} _{Tetragonal Centre Vibronics }
4.4 4.10 4.14 5.4 5.11
6.4 6.8
6.9
6.16 6.21
6._{35 }
6
.
37
6.386
.
39
8.5
vii
ABSTRACT
Both the optical and infrared spectra of cerium and
praseodymium tri_{}positive ions in the alkaline earth
fluorines have been studied. Various charge compensation
mechanisms have been employed including negative hydride,
deuteride and tritide ions.
For the hydride centres the degenerate local mode lines are resolved into more than one component. These splittings are attributed to electronphonon interaction effects between the low lying rare earth 4f electronic states and the hydride ion local mode phonons.
The 4f5d electronic transitions of the cerium hydride 1
type centres show large isotope shifts up to 50 cm . Only the nondegenerate hydride ion vibration appears in the 4f5d optical spectra and the vibrational interval is
increased from absorption to fluorescence by as much as 15%.
Both the isotope and vibronic shifts for the tetragonal cerium sites are attributed to electronphonon interaction effects.
C H A P T E R I
INTRODUCTION
1.1
In recent years considerable progress has been made in the interpretation of the vibrational spectra of light
impurity ions in crystals(1,2,3). The light ions vibrate at frequencies appreciably higher than those propagated by the lattice and so vibrational modes strongly localised about the defect ion are produced. These localised modes are observed, at low temperatures, as sharp absorption lines in the infrared. The number and frequencies of these lines and the appearance of harmonics is determined by the site
symmetry of the light ion. The linewidths and relative
intensities are determined by the coupling of the local modes to their environment.
Negative hydrogen and deuterium ions incorporated in the alkaline earth halides give rise to good examples of local ised modes and have been extensively studied(4)0
Similarly the electronic spectra of rare earth ions in
many host lattices are now well understood (5,6)_{. } _{The } 4fn  4fn1 5d transitions are observed in the ultraviolet
1.2
associated phonon sidebands. In suitable cases these phonon sidebands are resolved into peaks corresponding to peaks in the phonon density of states of the host lattice and to vibrational modes strongly localised in the vicinity of the rare earth ion. A representative example of these transit ions is that of trivalent cerium in the alkaline earth
fluorides whose spectra have been reported by Kapalanskii(?)
among others(S)_{. }
The most prominent zero phonon line in the three thous and angstrom region has been identified(_{g}) _{as a 4}_{f}_{5d trans} ition of cerium in a crystal field of tetragonal symmetry. In this case charge compensation is effected by an inter stitial fluorine ion located in an adjacent empty cube of fluorines in the fluoride lattice (Fig. 2). In this work it is shown that analogous spectra can be produced with hydride ions serving as charge compensators.
These centres have been previously studied by E.S.R. techniquesC10_{,}11) and the infrared hydride local mode absorption has been reported by Jones et a1. C12)_{. }
The effects of replacing the fluoride ion charge compen sator by hydride or deuteride ions have been discussed(
13)
for the gadolinium ion in calcium fluoride. New electronic lines are produced in the optical spectrum of the crystal as a consequence of the changed environment of the gadoliniumThe frequencies of these new electronic transitions are slightly different for H and D charge compensations. This frequency difference constitutes the electronic 'isotope shift'.
Vibronic transitions are observed whose vibrational frequency intervals match the frequencies of the H and D localised modes. Since the transitions involved in this work were ff (in this case 8s_{712 }  6F_{712) these vibronics were } very much less intense than their parent electronic transit ions.
The above effects were reported previously by Jones and SattenC14) _{in a study of H and D ions in the rare earth } trifluorides. They interpreted the isotope shifts (defined above) as due to a dynamic coupling between the rare earth and hydride ions. Unfortunately the small size of the effects and uncertainties about the crystal structure and site symmetries made a detailed comparison of theory with experiment impossible.
Imbus et a1. C
15)
_{report similar small shifts for the R } lines of chromium isotopes in ruby and magnesium oxide.The coupling between the optically active electrons of a defect ion and the lattice manifests itself in several ways.
(1) Through shifts in the energies of electronic transitions.
(2) By modifications of the lattice or localised vibrations.
(We are not concerned in this work with the des truction of electronic selection rules or with the lifetimes of excited states.)
In many cases these terms are small and/or the inter actions so numerous that the various effects, if observable, cannot be unambiguously identified. It is therefore useful to investigate simple experimental situations with well
localised vibrational modes where the electron_{}phonon inter action is not so strong as to preclude the observation of detailed structure and yet strong enough to give rise to
effects which may be accurately measured. Rare earth hydride ion pairs in the alkaline earth fluorides largely fulfil
these requirements.
The local mode infrared absorption lines are extremely narrow which allows the resolution of fine structure (Ch. IV). The positions of the low lying rare earth energy levels can be determined or estimated from the optical
greater than the previously observed intraconfigurational
isotope shifts. Similarly large vibronic shifts, defined as
the difference between the vibrational frequency interval for absorption and fluorescence spectra, are observed for the
local mode vibronic progressions. The system is also conven
C H A P T E R I I
A REVIEW OF THE THEORY
Lattice and Localised Vibrations
2.'1
If we suppose that the effects of the electrons may be represented as a static internuclear potential we may write the Hamiltonian which describes the atomic vibrations in a perfect crystal as:
Pc/(.e,k)
Jl
= _{E } _{___ ... }+
i
_{E } _{E } _{µ ( }tk)
<I> ,v A(
,ek ',e
Ik
I ) µ A (,e ' k
I ) tk2M(t,
k)
tka t'k'a' a �,.., ,..,( '1)
where p andµ are t_{a } _{a } he momentum and displacement of the kth atom in unit cell
_{,e, }
where a defines the cartesiancoordinates.
The elements of <I>a� are the socalled force constants and are the second degree coefficients in the Taylor series expansion of the crystal potential energy. Cubic and
higher terms in this expansion have been neglected.
The equations of motion are
M(.ek)u C.ek)
a +_{k't'� }
E <I> a,, AC.e
'
k
'
)µ
_{,.., }ACt
'
k
'
)
=o
Because of the periodic symmetry of the lattice the atomic force constants depend only on the intercell distance and the displacement amplitude may be written as
2.2
= e (k) a _{e }i(k.r.•wt) rv '""l
_{(3) }
The eigenvalue equation determining the relation between
w and k is found by substituting (3) in (2)rv . The resulting
solutions are extensively discussed in the literature(17
,
18)_{. } For each value of k there are 3� solutions where � is the number of atoms per unit cell. The � branches of the multi valued function w(k) for which w(k)  0 as k  0 are labelled rv rv rvacoustic and the remaining
3�3
branches optical since for an ionic crystal these modes impart a macroscopicfluctuating dipole moment which may interact with an incident electromagnetic wave.
This process is responsible for the restrahlen absorp tion characteristic of ionic crystals and gives rise to the strong infrared absorption of calcium and strontium fluoride
1
crystals in the 500 cm region. If the crystal were
perfectly harmonic the absorption spectrum would consist of delta functions. However, since the crystal is not
harmonic the delta function peaks are broadened into
Lorentzian peaks with sidebands corresponding to multiphonon processes.
If a point defect is introduced into the crystal the translational symmetry is destroyed and the normal modes of
2.3
The possible changes can be illustrated by considering a linear chain of identical atoms with a single mass
d f te ec (19,20,21) . If th f e orce cons an s are unc t t h ange d d an
the impurity mass is heavier as first shown by Rayleigh(22)
all the frequencies are lowered but not lower than the next
unperturbed frequency. If the impurity is lighter the
highest symmetric mode may be greatly displaced above the
band and forms the socalled localised mode since it cannot
be propagated throughout the lattice and is strongly
spatially localized about the defect.
Since the translational symmetry of the lattice is removed by the presence of the defects the selection rules governing infrared absorption are relaxed. Not only may
the localised modes be infrared active but also the slightly perturbed band modes give rise to new infrared absorptions which in the case of ionic crystals are superimposed on the
dominant restrahlen absorption.
One dimensional models have been discussed by several authors(23,24,25)_{_ } _{To obtain solutions for three dimensional } models Greens function techniques are employed. Extensions to the theory have been made by Dawber and Elliot(26) _{. }
Recent reviews include those of Maradudin(27) _{among }
others(2
s,
29)_{_ }2.4
model. These include the shell model(3o,3
1)
_{in which the } ions are represented as small heavy nuclei coupled by elastic springs to light rigid electron shells.Provided the impurity ion is significantly lighter than the lattice ions it can be treated as an anharmonic
oscillator in an effective static potential well. This
approach has been used successfully by Hayes et a1.C4,32) for
the case of H substitutional impurities in the alkaline
earth fluorides. In this case the H ion is in a tetrahedral environment and one second and two third harmonics are
observed. These observations provide sufficient data to determine the anharmonic constants which then allows the calculation of the positions of the forbidden second harmonics. These were later observed by the use of stressC33) _{in excellent agreement with the pr}_{e}_{di}_{c}_{tions}_{. }
Maradudin and Peretti(34) _{have examined the anharmonic }
oscillator in c_{4}_{v symmetry and have obtained a solution by } treating the cubic terms to second order and the quartic terms in first order perturbation. The first and second excited states of this oscillator are shown in figure (1).
The electric dipole operator transforms as r1+r5. in c4v and
�




,
1
2fuvz (002)
r
_{l }(101)
r
_{I }n(w_{xy}
Mvz)0
<011) 5 _{I }
<110)
r
4
� [(200) + (020)]1
_{1 } � [(200)  (020)]13
(001)
_{1}
_{1 }<010)
r
(100) 5(ooo)
f;_
I
j
I I
'
I
II
I J ! I ;!
I I Il
l I II
!
!I
I
l \I
l
I 1 1 l 2.52.6
This and several other point symmetries are reviewed by Newman(1 )_{. } _{This static well approximat}_{i}_{on}
, together with a large induced hydride ion dipole moment introduced by
Zdansky(35) _{in a study of Gd}3+_{}_{H tetragonal ion pairs in }
CaF2 is used in the interpretation of the spectra reported here and will be reviewed in detail.
The hydride ion is situated in an otherwise empty cube of fluorine ions adjacent to the rare earth ion (Fig. (2_{))}. The extra positive charge on the rare earth will result in a nonlinear polarization of the hydride ion which is
represented by a dipole moment directed in line with the rare earth (Fig. (2b)). This dipole moment is assumed to have a constant magnitude, independent of the hydride ion position. The effective static potential well in which the hydride ion is taken to vibrate can be written as the sum of cubic and tetragonal components:
=
V
_{+ }V
C tetg.
to third order
The dipole moment p will interact with this field through its gradient. From Fig. _{(2b) }
(a)
(b)
I
10
"��
, I ,,, I ,' I
I I 10 I
,,•..
,•
Fig (2).
F"
I ,©
,
�

�


, 1 ," I ,,.. IH '
Co2•0
I 0....}_ _{\...T'i } �0 _{RE3• }
,•  ,+  ,r,· .
, , I , I
10 I
,,• >·
'(
a • • Schematic representation of the calcium
5+
fluoride lattice showing the tetragonal Re
site with interstitial cho.rge compensators. b • • Schematic representation of the dipole
moment p of the H ion. _{;;.J }
2D  Th
1
ur1i t cell d.im<msion iFJ 5.'15 5.'"/8. .
_{£VVe } =V _{tetg } = � k
2Ap (x2_{+y}2_{) }
qD + � z(x_{qD } 2+y2)
k
p�(1) _{Y�( 8, cp) /}_{2}_{��1 }
CT V
Dk+1
2Ap
qD (z)
Expanding in terms of cartesian coordinates etc. gives
;12.vvtetg =
Which gives, on equating coefficients
a =
b =
C =
d =
� + _{D } 4p5a _{D }
2Ap qD
4pa 3Ap
5 + 2
D
qD
These expressions will be referred to as required.
2.9
The Electronic Levels of Ions in Crystals
The crystal field theory dates back to the work of Bethe(36) _{and Kramars}(37) _{and along with the theory of free }
ion spectra is well known, at least in general outline.
=
The free ion Hamiltonian may be written as:
fm
2 _{2 } _{2e}2 _{e}2� V.  E  + i E  +
i 1 i ri ifj rij
where the symbols have their usual meanings.
When the ion is embedded in a crystal lattice the spherical symmetry which characterises the free ion is
destroyed. H is no longer invariant under infinitesimal
rotations but only under the operations of the point group
which describes the site symmetry.
Provided that the electrons are sufficiently localised the effect of the ligands may be represented by a static potential V.
H = H_{f } + V.
We may distinguish two cases.
(1) Very weak crystal field having less effect on the energy
levels than the spin orbit coupling term. The f
electrons of the rare earths are 'shielded' by the 5s and 5p electrons and may be treated in this way.
2.10
the Coulomb interaction term. This case is appropriate for treating the excited 5d levels of the rare earths. The potential V may be conveniently written as a series of spherical harmonics
V = _{I: } _{I: Aq }]" k .
kq k l pkq (cos e.) l e iqcp. i where k = _{0' }
oo,
_{l}_{q }_{I }<
_{k } _{and the }_{summation is } all the 4f electrons. Fortunately only�fewcarried out over of t·he terms in this infinite expansion give nonzero contributions to the matrix elements between electronic states. The calculation of energy levels will involve integrals of the form
f 2 k 2 _{R4fr r dr }
ff
_{p3 p3 p}m' m" q i ( m" m'+ q) cp . _{k } e sin 8d8dcpk k
The integral over r gives <r > the average value of r. The integral over 8 and cp is zero unless k
<
6 for felectrons, k is even, and (m"m'+_{q) } = 0.
The Af are often defined in terms of Vf (Stevens 1952)
see table (Dieke). Alternately they may be expressed in
terms of tensor operators c�k) _{or spherical harmonics Yf}_{. }
+
vq
_{k }=
=
where the N(C(k)_{) } _{are normalisation constants}_{. } _{Since there } q
2.11
integrals the theory has been most successful if the Af<rk> are defined as a single coefficient Bf and the Bf taken as parameters to be obtained experimentally.
The matrix elements of V with electronic states
characterized by the quantum numbers SLJM may be evaluated by making use of the WignerEckart theorem
<a:JMIVfla:'J'M_{'}> = _{(}_{}_{1)}JM
(
J Mk
q M'
J')
<
aJI I
vk
II
a' J '>
The reduced matrix elements are independent of M and must be calculated for each pair of states. Tables for the
evaluation of Rare Earth f level matrix elements in both LS and coupling are given in
(5)
.
The lowest lying levels are in general fairly well isolated and the intermediate coupling effects are not large.Once the interaction matrices have been obtained they must be diagonalised to find the energy levels.
The resulting energy levels for various J values in crystal fields of cubic symmetry have been reviewed by Lea Leosk and Wolf(3s)
.
_{In fields of lower symmetry the }remaining degeneracies are lifted.
The ElectronPhonon Interaction
Following Jones and SattenC14) _{we write the interaction }
2.12
vev = E f. Q. + E g .. Q. ].. l l _{lJ }. . l.J ]. J Q. + •••
where the Q_{i } _{and Qj are normal coordinates of vibration of } the lattice and f and g are functions of the electron
coordinates.
For the rare earth, hydride ion pair in
c
_{4}_{v symmetry } this expression becomesVev = fxX + fYY + fzZ + i(g_{xx}+g_{yy})(X2+Y2)
+ f(gxxg_{yy})(X2_y2) + gxxX2 _{+ gyyY}2 _{+ gzzz}2
where X, Y, Z are the normal coordinates of the hydride ion displacement.
The crystal field potential may be expanded as a Taylor series in the light ion displacements to give
�avco�
1a
2vco
V c = V O + _{C } _{i i }E
ax
/SX.. 1 + 2 _{ij � j }Eax ax
/J.X. _{l. J }/J.X . + • • •T _{n,x }
T m _{n, y }
2.13
=
where r,
e, �
are the polar coordinates of the electron and m ( n where pnm(cos e) are the legendre polynomials.The Coulomb potential at r of a point charge at R can now be written down since for
lgl
>It!
IE;sl
= L M mR_{n } (2n+1)[T _{nx � n, x � + ny � n, y }m(R)T m(r) T m(R)T m( )]_{£ }
where M m _{n } = 2 fnmj; _{n+m . for m f 0 }
and M 0 _{n } = 1
This relation can also be used to derive the dipole moment 1
potential given by p.grad
lg£!
.
The resulting expressionsare somewhat lengthy and may be obtained from
_{(35)}
.
Differeptiation is greatly facilitated by the use of recurrence relations also given in(35)
.
V transforms as the totally symmetric representation _{ev }
of C _{oov } and the f. , g .. functions will transform as the same _{l } _{lJ }
irreducible representations as the corresponding functions
of light ion displacements. The following relations hold
between the solid harmonics and the f. and g ... _{l } _{lJ }
2.14
= = b T_{1n nx }1 _{Cg g ) }_{xx yy } = b _{2n nx }T2
0
c0 T n n = = c T2n ny 2
The constants a0n etc. will depend on the particular model chosen for the light ion interaction.
The simplest is the point charge model for which the potential of the cerium ion in the point charge field of the hydride ion is a function of the difference in the cartesian coordinates of the electron and hydride ion, so that:
=
av
C ax.
_{l }Using this together with the generating function for legendre polynomials,
=
gives the following values for the constants.
=
=
=
=
(n+1)eq D(n+2)
c _{On } = _{i(n+1)(n+2)eq } D(n+
3)
D(n+2)
eq
(n+2)eq D(n+3)
2.15
where Dis the separation, at equilibrium, of the hydride and rare earth ions. Since Laplaces equation is satisfied we have also
=
o
.
The corresponding constants for the dipole model are obtained
in the same way and their values are given by
aon = _{}_{(n+1)(n+2)epD}(n+3) a1n = _{}(n+3)epD(n+3)
bon = _{l(n+1)(n+2)(n+3)peD}(n+4)
con = _{½(n+1)[(n+1)(n+2)+2]peD}(n+4)
C H A P T E R I I I
EXPERIMENTAL CONSIDERATIONS
Calcium, strontium and barium fluoride have the same crystal structure, space group
at
.
The lattice may be vis ualised as the superposition of three face centred cubic lattices or, more usefully for this work as a simple cubic lattice of monovalent fluorine ions every second box of which is occupied by a divalent metal ion (Fig. 2). The crystals are ideal hosts for optical studies being transparent from the middle infrared to the far ultraviolet and nonhygroscopic. The samples used in ·this work were either cleaved along (111) planes or cut with a diamond saw and polished on a felt lap with tin oxide powder.
Rare earth ions can be incorporated at divalent cation sites when the crystals are grown from a melt containing both
metal and rare earth fluorides (Stockbarger method). Since
the trivalent rare earths have radii very similar to the ions which they replace no serious disruption of the lattice
takes place with rare earth concentrations as high as
5%
.
Some form of charge compensation is however required. Unless
precautions are taken this is achieved by the replacement of

2F by O ions. The addition of lead fluoride to the melt
The rare earth doped calcium fluoride crystals used were
purchased from the Hebrew University of Jerusalem, Israel.
Strontium and barium .fluoride crystals were obtained from
Optovac Inc. Nominal rare earth concentrations of 0.05% were found to be convenient in most cases and have been used
except where otherwise stated. At concentrations of 0.2% and above all spectral lines become broadened due to small
lattice distortions and in some cases the spectra become con
fused with many lines due to rare earth ions in a multiplic ity of lattice sites.
Hydrogenation
3.3
centres for calcium fluoride and one twentieth for strontium
fluoride. It appears(39a) that these centres are not formed
for rare earths near the end of the sequence for strontium
fluoride.
Tritium was introduced into the crystals in the same way at one tenth atmospheric pressure. A glass capsule containing two cubic centimetres of tritium gas was sealed into the
quartz tube and broken with a ball bearing and external mag net. Hydride centres were found to be present in all
crystals doped in this way in the approximate ratio (H:T )
of 4:�. The tritiated crystals became strongly coloured after several days due to the strong optical absorption of divalent rare earth ions produced by the low energy beta emission from the tritium. Baking at 300°_{c for several }
hours largely removed these centres and allowed optical
measurements to be repeated. Oxygen was introduced into the
as grown crystals by heating to 900°_{c in an o}
xygen atmosphere.
More complete conversion to oxygen centres is however effected by first hydrogenating the samples as above.
In addition to the two fluorides above barium and
cadmium fluoride and strontium chloride have the same crystal
structure and were considered as possible host materials.
Several attempts to obtain tetragonal hydride centres in
barium fluoride were unsuccessful. It has been noted by
also not readily formed in this material. Cadmium fluoride is attacked by molten aluminium and cannot be hydrogenated in the normal way.
Attempts to hydrogenate pure cadmium fluoride by heating to 600°_{C in an atmosphere of hydrogen and in the presence of } cadmium metal were unsuccessful. Strontium chloride cerium doped crystals were grown in this laboratory by R. Ritchie.
Since when subjected to the thermal shock required to quench hydrogenated samples these crystals became opaque and since the lattice constant is larger than barium fluoride for which no tetragonal centres could be formed, no effort was made to refine the growth techniques to remove oxygen impurities.
Instrumentation
Measurements were made in the 6003000 cm1 range with a Beckman IR12 infrared spectrophotometer providing a maximum resolution of 0.3 cm1 at 1000 cm1•
Optical spectra were recorded photoelectrically using a ¾meter Czerny Turner spectrometer made by Spex Industries
Inc. with a dispersion of eleven angstroms per millimeter in the ultraviolet. This instrument provided sufficient
For absorption measurements the dense filament of a one hundred watt quartziodine lamp was used as source from
25006000 A0 _{being replaced by a deuterium lamp at shorter }
wavelengths. Various Corning glass filters were used to re move unwanted spectral orders and were placed between the source and the dewar to reduce radiation heating.
Fluorescence spectra were obtained using a Philips 500 watt high pressure mercury lamp for excitation. Interference and glass filters were used to remove the scattered back
ground mercury radiation. This background proved particular ly troublesome in the case of cerium fluorescence. Best
results were obtained using a Bausch and Lomb monochromator as filter in spite of the considerable loss of fluorescence intensity. In this way selective excitation of sites could be achieved further reducing the background and hence improv
ing greatly the signal to noise ratio.
Low temperature optical spectra were obtained using a
variable temperature dewar made by Andonian Associates.
Cooling is achieved via thermal contact with a copper block,
in contact with the liquid (Helium or Nitrogen).
Low temperature infrared measurements were made with a
similar dewar fitted with cesium iodide windows. Thermal
contact between the crystal and copper block was improved by
Photoelectric rather than photographic recording was used throughout since this provides better reproduction of the structure of absorption bands and of fluorescence spectra with high background radiation levels. The absorption
C H A P T E R I V
EXPERIMENTAL RESULTS. PART ONE
Infrared Spectra
4.1
Several rapidly quenched hydrogenated crystals of
calcium and strontium fluoride containing cerium and pras.eo
dymium were examined in the infrared. Typical absorption
spectra obtained at liquid nitrogen temperature are reproduc
ed in figure 3. For each host the predominant tetrahedral
substitutional site absorption can be clearly seen at 965
cm 1 in calcium fluoride and 893 cm1 in strontium fluoride.
The previously reported local mode lines associated with rare earth hydride ion tetragonal pairs in calcium fluoride are reproduced and similar lines appear in the strontium fluoride
spectra. New tetragonal hydride ion sites correlated in in�
tensity with these lines in strontium fluoride have recently
been observed in this laboratory by ESR( 4o ) _{which confirms }
the assignment of these lines to tetragonal sites analogous
to those in calcium fluoride. This assignment was initially
made on the basis of the similarity of the optical spectra to
be discussed in later chapters. The two components are less
well separated in strontium .fluoride and the separation is subject to more fluctuation with change of rare earth o
On the basis of an approximate 2: 1 intensity ratio
. ' Pr H 3+  .
1 200 1 1 00 1 000 SrF2
�' I
I
Il
I i
I
I
.
4. 2
,
_{I },____,_I
___
L
______ l
1.
1 1 00 1 000 900
.Energy  cm1
series the broad high frequency line was assigned by Jones et a1.C12) _{to the doubly degenerate (x:y) vibration and the }
narrower low frequency line to the (z) vibration. However, as pointed out by Newman(1) _{and confirmed here}_{, } _{the ratio } deviates significantly from 2: 1 and for the first two members of the series is closer to 1: 1 (see table 1) . (The comparis on for cerium in calcium fluoride is made more difficult by the superposition of a combination band (lattice phonon plus tetrahedral site local mode) and the high frequency compon ent. The entry in table 1 has been obtained by subtracting this band, the intensity of which was determined by monitor ing the intensity of the second harmonic of 9650 ] The
assignment of modes on an intensity basis is seen to be at best tentative and some other means must be sought. Fortun ately this is available without resorting to stress or
electric fields to raise the degeneracy.
At lower temperatures and at high resolution the low frequency components in both host Jattices containing cerium have been themselves resolved into two components. Spectra recorded at 8°_{K are reproduced in figure 4}_{. } _{The crystal } temperature measured with a thermocouple clamped to the out side of the crystal is slightly above that of the liquid helium since a conduction dewar was used and some radiation heating occurred. _{The resolution of this line into two }
come 1
ce3+ Pr3+
cw2 1.0 0.9
SrF2 1.3 1 o 2
Table (1) . The relative intensities of the two infrared local mode absorption lines associated with each rare earth hydride ion tetragonal pair for cerium and
praseodymium. The ratio is quoted as :
4.4
993 992
920 9 1 .9
9 9 1
WA;6Ji. •
3+ . CaF Ce H _{2 }
990
Energy  cm 1 •
9 1 8 9 1 7
Energy  cm1 .
·1
I
989
9 1 6
J?i g ( '1· ) • Hi gh r e oolu ti on i nfrared ab sorption apeo tra
showing ol early the ( xy ) hydride ion locnl moclc
vi bration apllt by the order pf one wave number . In each caoe the affects of noi se have been minimi sed by tho
superposi tion of eovoral traces. Temperature 8 K. _{. } 0
 1
20°_{K) listed in (}_{1}_{2}
) without comment. The high energy line
remains unsplit (at least with the resolution available) and appears as a single line only a little wider than a wave number in strontium fluoride.
Small splittings observed for both components of the analogous erbium and ytterbium centres have been discussed by Newman and ChambersC 41 )_{. } _{They have established a mechanism } for the splitting which involves a thermally populated rare earth electronic level close to the ground state. Cerium is not expected (Ch. VI) to have an excited level below one hundred wavenumbers and since the two components maintain their relative intensities down to 4°K this mechanism cannot account for the splitting in this case o The above mechanism would also be expected to produce a splitting of the high frequency line which is not observed.
The situation is more involved in the case of praseo dymium centres. The corresponding low temperature high resolution spectra are reproduced in figure
5
.
Again thelow frequency line is resolved into more than one component and the high frequency line remains unsplit. The overall intensity ratios of the (xy) and (z) components are very
similar to the cerium values but the low frequency line does not show the same simple two component structure. The
corresponding pattern in strontium fluoride is apparently
4.7
1
,

·· ··. ___.. .... 
_{J }
_{" }
/1
I 3+  i
l
Ca�2Pr H iI
f 1 00 1
i
92
Fi g. ( 5) .
1 000 999
I I
998 9 97 996
1
Energy  cm
995
SrF Pr3+ _{}
H2
994
925 9 24 9 2 3 9 22 9 2 1 9 20 9 1 9 9 1 8
Energy  cm  1
High resolution infrared absorption suec tra
showing the splitting of the ( xy) fourfold degenerate
H local mode. Temperature 8°_{K }
 1
4.8
Similar splittings have not been observed for the other
rare earths. For example, in calcium fluoride, neodymium
hydride centres show only a single symmetrical line at
similar resolution down to 4°_{K}_{. } _{The linewidth , 0}_{.}_{9 cm1, is }
similar to that of the individual components above .
It is apparent that the splitting in both magnitude and number of components is closely dependent on the rare earth concerned and that the magnitude of the splitting is in some cases closely dependent on the host lattice. Both these
observations suggest that the effects are due to interactions involving the local modes and the low lying energy levels of the rare earths.
Vibronic Levels
Since the hydride ion is much lighter than the lattice ions the static well approximation may be used and since the anharmonic terms are relatively small the nuclear wavefunctions may in first order be written as the product of three one
dimensional harmonic oscillator wavefunctions, normal
coordinates x, y and z. Since the electronphonon interact
ion is small the wavefunctions of the combined system (i.e.
vibronic wavefunctions) may be written in the BornOppenheimer approximation as products of the form
�in =
where �i is an electronic rare earth wavefunction and �n is
4
.
9
Both the rare earth and hydride ions occupy sites of point group symmetry
c
_{4}_{v}. The properties of this group are well knownC 42) _{and its multiplication table is reproduced in } table 2. Both the electronic and nuclear wavefunctions willtransform as particular irreducible representations of this group.
Since the cerium ion has a single 4f electron the
relevant electronic wavefunctions will have halfintegral
angular momentum and transform according to either the
r
_{6 or }r
_{7 representation of the }c
_{4v double group}. The first excitedstate of the harmonic oscillator transforms as
r
_{5 }
and thusthe combined vibronic wavefunctions will transform as
= _{i } = 6 , 7
Thus in principle the electronphonon interactions V ev
may split the (xy) vibronic level into two components. The
(z) vibronic level will transform as
=
r.
l i = 6 , 7
and thus cannot be split. Since the splitting occurs for the low frequency components in fig. 3 it is therefore concluded that these must be identified as the (xy) vibronic levels.
r1
_{r2 }
_{r3 }
r4
_{r5 }
_{r6 }
_{r7 }
r1
r2
r3
r4
_{r5 }
_{r6 }
_{r7 }
_{r1 }
r1
r2
r3
r5
r6
r7
r2
r
_{.., }_{r2 }
_{r5 }
_{r7 }
_{r6 }
_{r3 }
r 1
r5
r7
r6
r4
r1+r2
_{r6+r7 }
_{r6+r7 r5 }
+r3+r4
r1+r2 r3+r4
+r5
+r5
r6
r1+r2
I'7
+r5
Table
(.gl
.
Multiplication table of thec
_{4v double group }4.1 1
The remaining odd electron rare earth ions including neodymium will also produce vibronic levels transforming as r6+r7 and in principle Vev may split these levels. The absence of observable splittings for neodymium etc. will be discussed in Chapter V
In contrast praseodymium has an even number of 4f
electrons and so the electronic wavefunctions will transform as rj of
c
_{4v where j = 1 } . • • 5. If the ground state trans forms as ri i=
1 .. • _{4 then since rixr5 }=
_{r5 and rixr1 }=
_{ri }both the (xy) and (z) vibronic levels will give rise to
single absorption lines. If however the groundstate trans forms as r5 then since
=
the (xy) vibronic level may in principle be split into four. Since the vibronic is split we conclude that, in agreement with the estimate of Weber and BierigC57)_{, } _{the r5 electronic }
4.12















;
I
i
(!)
0 ; P l
� .o _{f:1 ' }I
o i
U) I ,0 <! I
l :
999
 Calculated envelope of three lines.
>< x x Experimental points.
  Indivi dual lines. ( See table below. )
Fig ( 6 ) above. Computer generated least squares fit of three Lorentzian lines to the infrared absorption spectrum associated with the low enere;y H local mode vibration. Pr3+_{H tetragonal }
c0nters in CaP_{2}• Temperature
s
°K
.
Resolution 0. 3 c�1•I
.
Peak position.! _{cm 1 }
I
Width.
cm1 Relativo intensity
I
.I
,__ ______ __._ ____ +


1
999 . 5 ( 5 ) 1 . 2( 0 ) 1 . 0
996.7 ( 2) 0 . 9 (0)
996.1 ( 0 ) 0._{9 (5 ) }
4.13
The corresponding deuteride and tritide ion charge com
pensated sites have been observed in the ultraviolet
(Chapter VI). Direct observation in the infrared is
difficult because of the strong absorption of the host
lattices in the appropriate regions. The situation is more
favourable in the strontium fluoride case but the strong carbon dioxide absorption at 670 cm1 interferes with the
observation of the low frequency deuteride component. Both
components were however located by Jones et al. (12) for
3+
Gd D tetragonal centres in CaF2• Since decay via two
phonon processes is possible, they were both 3 cm1 wide even at low temperatures. The observation of fine structure will therefore be more difficult in the deuteride case.
4.14
Crystal Temp
( 8°K) Mode
3+
CaF2Ce H _{w }
w _{z }
3+
SrF2Ce H _{wxy }
wz
CaF Pr3+ _{}_{}
H2
w _{xy }
w _{z }

·
3+
SrF_{2}Pr H
w _{xy }
w _{z }
3+
CaF2Ce D w _{z }
3+
SrF_{2}Ce D w _{z }
,.
Frequency (cm1)
t
99
_{991}0
_{.},
0
3
1131. 5
{
9
_{91}17
_{8},
_{.}_{6 }5
957.7996.1
9967
999.5
111_{7}.3
f 921.
5
l
922.9939.7
817.8
696 03
Linewidth
(cm1)
0.7
0.7
6 0 5
0.7
0.7
1.4
0.9 0.9
1.2
7
.
5
1.2 1.0
1.2
3.7
4.3
Relative
intensity
1 . 0 1.0 2.0
�
.
o
1.0 1.6 1.0 2.0
1. 0 4.8
3.0
1.0
3.4
. . .
. . .
Table
(
3)
.
Infrared absorption measurements for thetetragonal, rare earth , hydride ion sites.
C H A P T E R _{V }
A DISCUSSION OF THE INFRARED SPECTRA
PART I: Vibronic Splittings
CeriumHydride Centres
To estimate the magnitude of the splittings to b e ex pected we must evaluate the first and second order perturbat ions of the vibronic levels by the electronphonon interact iono We write:
= f
X
_{+ } fY
_{+ } fZ
_{+ } _{• • • }_{+ } f(g g) (X
2 2Y
)
. . .
X
y
_{Z } _{� }n
First order interactions involving the first degree terms in V will be zero since the nuclear parts of matrix _{e}_{v }
elements between the v_{ibronic levels are zero for the }
harmonic oscillator. First order interactions involving the second
degree terms will also not contribute to a splitting since,
for example, (gxxgyy) transforms as
r
4 ofc
4v and the directproduct
r
_{7}xr
_{4}xr
_{7 does not contain }r
_{1}• The electronic partsof the matrix elements will therefore be zero. The first
non_{}zero contribution will arise from the first degree terms
in V acting in second order via intermediate _{eV } vibronic
states as follows.
5. 2
..•�.,....,_., ,.._. _____ ,.,,,...w ... Jvl!.,TO':/" w� .. rn...,w
.\ '
\
\
J
I
I
I
I
I
\\ ___ ri,
\
'3
I
I:
I
I
I
I
,w
I
I/4
r;
_{>   rs }
r;
I
I
I
I
I
_{I }
I
I
.
E
G __ r:;_? __ ,' __f/
I
I
I
I
r;
'
IE l e ctr o ni c
stat e s
Vi b ro n i c
st at e s
\
\
\
\
\
\
 ri
p h o n o n
st at e s
'
l
,_.
________
"

...
.
=  [f X + f X ) + _{+ } _{ + } • • •
The f+ etc. transform as particular rows of
r
5
and we need now only calculate diagonal matrix elements. If a,� are electronic wavetunctions transforming asr
_{6 and 6},y asr
_{7 we } may list various products which have the same transformation properties (see table 4).The low lying electronic, vibrational and vibronic states are shown in figure
7
.
Using standard second order perturbation theory and taking into account all the intermediate vibronic levels of the appropriate symmetry the shift of the
r
_{7 }
level from its unsplit position is :<y(100) I V !6'_{(110)><6}1 _{(110) I V } _{l}_{r(100)>/(E�}_{, }
E0+?w)
ev · ev u
+ <r(100)
1v
! 61_{(000)> <6'(000) }1v
_{l}_{rC 100)>/CE�}_{,}_{}_{E0}_{}_{?w) }ev ev u
+ E <y(100) !V l a' Js.2[±)><a ' �2[±) 1 V l r(100)>/(E , _{E0+?w) }
+ ev v c:.. v c:.. ev a
where [±) = [(200) ± (020) ] and a similar expression holds
Evaluating matrix elements of the form:
<(100) I X+ l(OOO)><(OOO) IX_ l(100)> = 
?l2mw
etc.r6
r7
(X � 6 y
yX_ 6X+ 'YX _{+ } 6X
�x+ aX

_{�x}_{_ } _{aX+ }Yf 6f _{+ } _{yf+ } 6f
�f+ af

_{�f }
_{af+ }6[+] Y[+] a [+] � [+]
6[] Y[] a[ J �[]
where [±] =
°V2
1 [ ( 200) ± (020) ]Table (4). The transformation properties of the cerium,
hydride ion vibronic levels. Each entry in a column transforms in the same way (see page
and
=
2�w [ < y If_ I o' > < o' If+ I y > / ( E O, Eo + ?W) + <r I f_ I o ' > <o' _{If+ I r>/CE0}, _{E0}?w) J
+ ..i [<r I f I ex' ><ex' I f I y>/(E , _{mw } _{+ } _{} _{ex } _{E0}+ ?w) J
+ <y I f I ex' > <ex_{+ } ' I f I y>/(E , _{} _{ex } _{E0}1iw)J
+ mt [<rlf_ l o' > <o' \_{f+} l_{r>/(E0}, _{E0+?}w)J
The difference in these two values gives the desired splitting.
� E = ¾w[2i <r lfx \0' > <01 lfy lr>(1/(E0, E0_{}?w) _{} 1/(E0, E0+?w))
 2i <rl_{fx}l ex1 _{> <}_{ex}_{' }_{l f}
ylr>(1/(Eex, E0?w)  1 /(Eex, E0+?w))J
where the matrix elements are written in terms of f and f . _{X } _{y }
The greatest contribution will come from those intermed_{}
iate vibronic states which lie closest to that of the local
mode phonon. For the cerium case these energy levels have
been shown in figure
7
_{and their }_{energies } _{are discussed } inChapter VI. The two states are, in terms of _{IML Ms> ' }
\2_{F5}
/2'r7> = � 1 +2 , +f> + � \+2,±t>
+ _{� } 1 ±1 , ±t>
 m
1 ±2, +i>= _{'{377 }
IO+i> 
V477
_{1 +1, tl> }similarly the ground state wave function is the !2F_{51}_{2}
, r
_{7}>
Kramers doublet given by :2
� 1 +2 , +i> 
PJ
1 +3, tl>I
F _{5/2 ' r7> } =5.6
+
F2
I
±1 ' ±i>  �I
±2 , +i> (see ref. 43)We may obtain an estimate of the order of magnitude of the splitting by using these wavefunctions and the point charge model outlined in Chapter II. The matrix elements given in the expression for �E above are non zero only for a_{1}_{2 } and a_{14 }_{in the point charge expressions for fx and fy } given in Chapter II. These matrix elements are:
and
Using the point charge values of a_{12}, a_{14 ; } the values of <r2> and <r4
>
given by Bron( 44 ) _{and the energy level separat}ions given in Chapter VI (Fig.
7)
gives the contributions to the xy splitting as 5.2 and 0.2 cm1 for the r_{7 and } r6derived states respectively. The net splitting of
5
cm1 isin reasonable agreement with the observed value considering the limitations of the point charge model and shows that V _{ev }
5.7
The corresponding intermediate levels for strontium
fluoride have not been found but a comparison with other rare
earth ions in the two lattices indicates that the excited
( �) level probably lies about 450 cm 1 above the ground state.
This reduction in separation is largely compensated for by the reduction in local mode frequency. This coupled with the relative insensitivity of the splitting to the exact
energy difference leads to a predicted reduction in splitting of only 5%. Including a small increase in the value of D
(fig. 1) the point charge model leads to an expected value of the splitting in strontium fluoride of about 90% of that in calcium fluoride in good agreement with experiment (Table 3).
Other contributions to the splitting will arise due to second order interactions via the remaining 4f levels. These
2 _{1 }
are the F712 levels (Chapter VI) which lie about 2000 cm
above the ground state. Using the wave functions given in
(43) their total calculated contribution is of the order of
1
0. 1 cm and they may thus be neglected. Similarly second
and higher degree terms in V _{ev } acting via intermediate vib
ronic states involving ( z) as well as (xy) phonon states in
all cases give contributions tco small to account for the observed splittings.
The dipole model, outlined in Chapter II, gives a
further contribution of 6 cm 1 taking a12 = 5ep/D5 _{and }
Praseodymium Hydride Centres
The calculation of the local mode splitting in this case proceeds in the same way. There are however many more contri
butions since the 7H4 ground state splits into seven levels in a tetragonal field (figure 8). The second degree terms of Vev can also contribute in first order since r
_{5}
xrixr_{5 }
wherei = _{1 } _{• • • }_{4 contains r1 and so the electronic parts } _{of } _{the } matrix elements need not be zero as above.
To determine the expected splitting pattern we shall first evaluate the dominant second order contributions as above, followed by the first order effects due to the second degree terms in V _{ev }•
The wavefunctions of the doubly degenerate r
_{5 , }
3
_{H4 }groundstate of the praseodymium ion in terms of
I J
_{Mj > states } are:¢
+ =Yi
_{1 +3> }
Yi
_{1}

_{1 > }
=
Vi
_{l}

3>
_{}
Yi
_{1 +1 > }
_{(45) }Forming vibronic wavefunctions as products of these states with the (100) and (010) vibrational wavefunctions gives the following states which transform according to part
icular single ialued representations of
c
_{4v}. 1+ i¢�(100)]
¢1 =
V2
[¢a(010).
.
.
¢2 =
V2
1 [ ¢a(100)  i¢�(010)].
. .
r1'}oo c....,,
   _{1 }_{I }_{[ }_{f t I }
1.>
_ 1 rs
1G>

r
_{s},
1
, "?'
Fig ( 8 ) .
Approximate energy level diagram for
3+ 3+
the Pr ion ( P.c
n
tetg. centres) basedon the availible F and
o
2 site data.( Chapter Vlll ).
=
=
where _{<l>}_{a; } =
</>� =
1 ( + )
V2
<I> +</>V2
(<I>+ <1> )The wave functions of the excited levels of the
ground state are given by:
_{( 45) }
=
=
=
=
=
=
1 1
V2 1 2)
+_{V2 1}

2>
/;kl 4>  !J.1 0>
+/;1. l 4>
1
V21 4>

ft l 4>
1
ys l ±3>
+Yi 1 + 1>
/J+.1 4>
+/;J_ 1 0>
+/J.l 4>
1 1
y2 l 2>  f2 l 2>
5.10
3H
_{}4where the first
r
signifies the cubic state from which theyare derived.
We may draw up a table of all the relevant intermediate vibronic states which transform according to particular
single valued representations of
c
_{4v (table }5)
.
Each vibronic wave function </>i will be shifted by second order interact
ions , (via the first degree terms in V ) with each state in _{ev }